Evaluation of the formability of AA2198-T3 Al-Li alloy in warm sheet hydroforming

This study aims to investigate the formability of the AA2198-T3 Al-Li alloy in hydrodynamic deep drawing (HMDD), through experimentation and finite element simulation. The effects of the most critical factors were studied: die cavity pressure and forming temperature. The Gurson−Tvergaard−Needleman model (GTN model) was employed to analyze the formability of AA2198-T3 Al-Li alloy and predict the fracture in the hydroforming of a cylindrical part. Both the numerical and experimental results showed that the increase of the pressure inside the liquid chamber, within a certain range, contributes to improve the formability of the alloy. Increasing the temperature would reduce the required pressure for sheet hydroforming. Notably, the appropriate chamber pressure was beneficial to form good quality parts with a relatively uniform wall thickness. By analyzing the fracture morphologies, the brittle fracture of AA2198-T3 plays a main role at room temperature, but the ductile fracture was shown at the elevated temperature. must be declared. 7. The data that support the findings of this study are available from the corresponding author upon reasonable request.


Introduction
With the rapid development of the aerospace industry, modern military and civilian aircraft have developed towards high-speed overload, long life and flight safety. The materials and weight requirements of aircraft structural parts have become increasingly stringent. Aluminum-lithium (Al-Li) alloys offer great superiority for use in aircraft structure since they reduce the density, increase stiffness, increase the resistance to fracture toughness and fatigue crack growth, and enhance the corrosion resistance [1,2].
With the addition of lithium, the weight (density) of the alloy reduces approximately 3% for each 1% lithium addition to aluminium, while Young's modulus increases about 6% [1,3].
AA2198-T3 Al-Li alloy, as the third generation of damage-tolerant Al-Li alloys, is considered as one of the most competitive lightweight and high strength structural materials in the aerospace industry [4][5][6][7]. However, the application of formed parts in critical structures is still restricted by the material low formability at ambient temperature [8][9][10].
Owing to the technical advantages of high forming limit, high dimensional precision, and good surface quality, hydrodynamic deep drawing (HMDD) method is widely used in the forming of complex thin-walled parts, especially aluminium alloy parts used in the aerospace field [11,12]. In the process, filling chamber instead of the original die, the pressure on the sheet comes from the liquid medium instead of a rigid die, hydraulic pressure to promote the formation of sheet metal. Under the action of the liquid chamber pressure, the plate and the punch fit closely, and the friction effect reduces the tendency of the plate to break at the corner of the punch; at the same time, the radial tensile stress is effectively reduced, and the wall thickness uniformity of the plate is improved. In addition, when the pressure of the liquid chamber reaches a certain value, the hydraulic pressure lifts the sheet material, and the liquid can flow between the sheet material and the die and blank holder. The lubricated function reduces the deformation resistance of the flange and the friction between the sheet and the die, improving the surface quality of the part. However, the application of Al-Li alloy formed components in critical structures is still restricted, due to the low formability at room temperature. Warm hydroforming provides a good solution since the elevated temperature can increase the flow of the metal [13]. Fig. 1 shows a schematic representation of the warm HMDD process.  Therefore, the subject of the present paper was to study the characteristic of plastic deformation of AA2198-T3 alloy in the warm hydroforming. Meanwhile, the effect of the process parameters on the fracture behavior in the hydroforming process was numerically studied, employing the GTN model.

Uniaxial tensile tests
Uniaxial tensile tests were conducted on a STM5000 testing machine. The sheet specimens of AA2198-T3 Al-Li alloy with the thickness of 2.0 mm were cut along the rolling direction. The deformation behavior at ambient temperature and 423K were measured under the strain rates of 10 −3 s −1 , 10 −2 s −1 and 10 −1 s −1 . Considering the effect of strain and strain rate on the flow stress of the material, Fields-Backofen [19] constitutive equation is often used to describe the stress-strain relationship of materials under different deformation temperatures and different strain rates. The parameters of the Fields-Backofen equation shown in Equation (1) are obtained through isothermal experimental testing. Parameter fits and is listed in Table 1.
=̇ (1) where K is strength coefficient, n is hardening exponent and m is the strain rate sensitivity exponent.
In the equation, K, n and m are constants of the material at a certain strain rate and a certain deformation temperature, that is, the values of K, n and m will change with the changes of temperature and strain rate. K, n, m and strain rate and temperature T mathematical relationship.
The hardening exponent-n is as followed.
From the deduced formula, it can be found that at a certain temperature and a certain strain rate, the strain hardening exponent n is the slope of the straight line in the   ln ln  coordinate plane. The stress-strain logarithmic relationship curves at different strain rates were made for each temperature. Take the plastic deformation stage curve fitting to obtain a straight line, and find the slope of the straight line, that is, the hardening exponent n.
The strain rate sensitivity exponent-m is as followed.
The strain rate sensitivity exponent-m was determined using a constant strain rate stretching method. At a certain temperature, stress-strain curves obtained at different strain rates are plotted in the same coordinate system. Select the uniform plastic stage, obtain the stress-strain coordinate point and take the natural logarithm, draw the coordinate points in the same coordinate system and perform linear regression fitting to obtain the curve. The slope of the straight line is the m value at the temperature.
The strength coefficient K at each temperature was determined from the calculated values of m and n, respectively.

Sheet hydroforming tests
Hydrodynamic deep drawing experiments were carried out to evaluate the formability of AA2198-T3 Al-Li alloy in warm sheet hydroforming at the double-action hydraulic press. The diameter and thickness of the initial sheet blank was 127.6 mm and 2.0 mm. The fillet radius of punch and die were 10 mm and 8 mm respectively. The blank holder gap was 1.1 times the sheet thickness. Fig. 2 shows the experiment equipment of the warm HMDD.
Firstly, the liquid cavity was fully filled with hydraulic oil under high temperature (≤573K). Then, the sheets were put on the die surface and the blank holder gap was kept fixed, at 2.2 mm, through walking beam of the double-action hydraulic press. By heating the tools and the hydraulic oil, the sheet reached the required temperature. The punch started the downward movement, to press the sheet into the cavity, once the temperature indicator reach the required value, and the pressure of the liquid chamber was controlled by using the pressure control valve.

GTN damage model
Based on the microscopic void theory, the fracture of metals includes three stages, namely void nucleation, void growth, and void coalescence [20]. Gurson [21] proposed a continuum damage model according to the theory. The yield condition is shown as follows: where q is the macroscopic von Mises equivalent stress, σ y is the current flow stress of the matrix, p is the macroscopic hydrostatic stress, and the function f * (f) models the rapid loss of stress carrying capacity, which accompanies the void coalescence. This function is defined in terms of the void volume fraction as follows: In the above relationship, is a critical value of the void volume fraction, and is the value of void volume fraction at which there is a complete loss of stress carrying capacity in the material.
Damage evolution in the metal includes two stages, void growth f g and nucleation f n : The growth of the existing voids is based on the law of conservation of mass and is expressed in terms of the void volume fraction: where ε̇k k p is hydrostatic component of the plastic strain rate tensor.
The nucleation of voids is given by a strain-controlled relationship: ) where f N is the volume fraction of the nucleated voids and voids are nucleated only in tension. The normal distribution of the nucleation strain has a mean value ε N and standard deviation S N , ε e p is the von Mises equivalent plastic strain, and ε̇e p is the von Mises equivalent plastic strain rate.
According to the recommendations found in the literature of Needleman and Tvergaard [22] and Benseddiq and Imad [23], the values of some parameters in the present study have been adopted as follows: q 1 = 1.5 , q 2 = 1 , q 3 = q 1 2 = 2.25 ,  [24][25][26]. The tensile test of AA2198-T3 alloy specimen have been simulated using Abaqus finite element code. Consequently, the parameters of GTN model for AA2198-T3 at different temperatures were obtained as shown in Table 2.

Deformation behavior and formability
The distribution of the equivalent plastic strain predicted by the FE simulation model under different hydraulic pressures at 298 K and 423 K are depicted in Figs. 4b and 4c respectively. The fracture occurred on punch corner or cylinder wall, when the pressure is not enough. Hydraulic anti-expansion can effectively prevent wrinkling of the sheet material at the corners of the die, and plays an important role in improving the forming accuracy of the part and increasing the forming limit of the sheet.
The formability at the room temperature can be improved as hydraulic pressure increases but still hard to form a completed cylindrical part as shown in Fig. 5. However, in warm hydroforming conditions it is easier to obtain good quality components, compared with forming at room temperature as shown in Fig. 5. The maximum draw depth was 35.4 mm at 298 k. Since the depth of the cylindrical part was not increased too much, the hydraulic pressure does not play a big role at the room temperature. As depicted in Fig. 4b, it can be seen clearly that the fracture occurred at the wall where high uniaxial tensile stress exists. It is difficult to draw a cylindrical part without cavity pressure. In other words, conventional deep drawing is not suitable for AA2198-T3 alloy.
When the forming temperature of 423 K was utilized during the process of HMDD, it is obviously seen in Fig. 4c Fig. 6. With the increase of hydraulic pressure, the thickness distribution becomes nonuniform. In zone I, the thickness distribution is relatively uniform. In zone II, the overall thickness distribution is not uniform, and the thickness variation is large; however, with the increase of hydraulic pressure, the thickness change amplitude decreases; at 25 MPa, the thickness distribution at 423 K is more uniform than 298 K.
In zone III, the thickness increased obviously as true distance form the cup center  The formed parts obtained from the HMDD experiment are shown in Fig. 7. The cylindrical part cannot be formed completely at the room temperature by using the HMDD. However, hydraulic pressure could improve the depth. The elevated temperature would improve the formability at 25 MPa hydraulic pressure since the deformation resistance of the blank flange decreases, which favors the material flow.
Comparing with the experimental results, the fracture generated from FE simulation at zone II is consistent.   Fig. 9. The force for warm HMDD is much lower than that for cold HMDD. In addition, the actual drawing force was greater than that obtained from FE analysis, which may be caused by friction between punch and seal ring on blank holder. The formability of AA2198-T3 Al-Li alloy is not good at room temperature. The HMDD process with proper fluid pressure can improve the formability of the alloy. The formed depth promoted with the increase of hydraulic pressure, but there is an optimal hydraulic pressure value beyond which the sheet will wrinkle. The fracture will occur after the pressure is up to a certain value at room temperature.
By utilizing the warm HMDD, the formability of A2198-T3 Al-Li alloy was much improved at the elevated temperature (423 K). The hydraulic pressure has a significant influence on the warm HMDD. When the hydraulic pressure reached a certain value (25 MPa), the formability is higher. Besides, the thickness distribution is more uniform at 423 K than at room temperature.

Microstructure and fracture mechanism
The microstructure and fracture of AA2198-T3 Al-Li alloy after HMDD was observed by Hitachi TM-3000 Tabletop Scanning Electron Microscope. SEM specimens were cut from the fracture region of the part at different temperatures with 15MPa.
From the SEM images in Fig. 10 (a), there is a large and smooth micro-fracture surface with a few dimples. At the high magnification ( Fig. 11(a)), the dimples barely exist. Therefore, the brittle fracture plays a dominant role at room temperature, appearing the poor ductility.
Meanwhile, at the elevated temperature of 423 K, the micro-fracture surface presents a fibrous structure in Fig. 10 (b) which is a typical characteristic of ductile fracture. Furthermore, many dimples and a large number of voids appear in the microfracture surface that demonstrate good plasticity as shown in Fig. 11 (b). The deformation should be the result of the combined action of grain deformation, grain dislocation movement and grain boundary movement. When the action cannot be eliminated, stress concentration will be generated. At this moment, micro-voids will appear in the grain boundary. As micro-voids coalesce together, the ductile fracture begins to initiate. Besides, the distribution of dimples is uneven and the dimples are small and shallow. With the increase of temperature, dimples increase and become more homogeneous. When the hydraulic pressure is 15 MPa, the void volume fraction at 298 K and 423 K were shown in Fig.12. At 298 K, when the pore volume fraction reaches 0.147, near the ultimate fracture void volume fraction of 0.15, the AA2198-T3 Al-Li alloy begins to break. This is consistent with the parameters of the GTN model shown in Table 2. However, with the liquid temperature rises to 423 K, the ultimate fracture value of the void volume fraction increases to 0.4, the material will fracture. As the liquid temperature rises, the fracture limit of the void volume fraction also increases.
Therefore, the forming depth of AA2198-T3 Al-Li alloy is also significantly increased.
From the void volume fraction, it can be seen that the fracture is likely to occur at punch corner or cylinder wall of the product, which is consistent with the results of the plastic strain cloud diagram. By analyzing the SEM images, the brittle fracture of AA2198-T3 Al-Li alloy plays a main role at the room temperature. The ductile fracture was shown at the elevated temperature. The GTN model can reflect the fracture behavior through calculating void nucleation (Fig. 13) and void growth (Fig. 14), which can be confirmed by the SEM images of AA2198-T3.

Conclusions
In this study, the formability of warm hydrodynamic deep drawing (HMDD) of AA2198-T3 Al-Li alloy through experimentation and finite element simulation was investigated. By using GTN model, a 3D FE model of the HMDD of A2198-T3 alloy sheets was developed at different temperatures. The effect of hydraulic pressure on HMDD process, formability and thickness distribution were studied. The main conclusions can be drawn as follows: (1) It showed a very poor formability of AA2198-T3 Al-Li alloy at room temperature. The HMDD process with proper fluid pressure can improve the formability of the alloy. The formed depth promoted with the increase of hydraulic pressure. However, the fracture will occur after the pressure is up to a certain value at room temperature.
(2) By utilizing the warm HMDD, the formability of AA2198-T3 Al-Li alloy was much improved at the elevated temperature (423 K). The hydraulic pressure has a significant influence on the warm HMDD. When the hydraulic pressure reached to a certain value (25 MPa), the plasticity can be much raised. Besides, the thickness distribution was more even at 423 K than the room temperature.
(3) By analyzing the SEM images, the brittle fracture of AA2198-T3 plays a main role at room temperature. The ductile fracture was shown at the elevated temperature.
The GTN model can reflect the fracture behavior through calculating void nucleation, void growth, and void coalescence.